International Journal of Trend in Scientific Research and Development (IJTSRD) Volume: 3 | Issue: 2 | Jan-Feb 2019 Available Online: www.ijtsrd.com e-ISSN: 2456 - 6470 Theoretical Study of Thermodynamic and Elastic Properties of Ti50Be34Zr16 BMG – A Pseudopotential Method Alkesh L. Gandhi1, Aditya M. Vora2 Professor, 2Associate Professor of Physics, B. V. Shah (Vadi-Vihar) Science College, C. U. Shah University, Wadhwan, Gujarat, India 2Department of Physics, University School of Sciences, Gujarat University, Ahmedabad, Gujarat, India 1Department 1Assistant ABSTRACT Pseudo-Alloy atom model under pseudopotential concept is effectively exploited to determine the elastic and thermodynamic properties of a bulk metallic glass (BMG). Such a study helps in finding novel applications of BMG. Here, the vibrational or phonon dynamics of BMG has been theoretically studied in terms of longitudinal and transverse mode of phonon eigen frequencies. The electron-ion interactions are represented by a well-established model potential with widely accepted local field correction functions. The computed results of the phonon dispersion curves (PDC) produce respective phononic nature in the amorphous glassy alloy. Keywords: Bulk metallic glass, Model potential, Phonon dispersion curve, Thermodynamic properties, Elastic properties 1. INTRODUCTION The discovery of bulk metallic glasses (BMGs) has encouraged extensive research interest because of their exciting technological potentials for novel applications and scientific importance in understanding their unique properties like high fracture strength, soft magnetism, excellent corrosion and wear resistances, anomalous electronic transport properties etc. BMGs have become popular as the new engineering materials in several applications extended from the common window glass to sports materials, prosthetic devices, scientific instruments, fashion jewelries, data storage devices in digital media, cellphone case, outer body of space vehicle etc. A BMG displays liquidus temperature below melting points of its configurational elements and behaves as an atomically frozen liquid, which forms a unique amorphous atomic structure of a glassy solid having high yield strength and high elastic limit under shock impact conditions as it is lacking slips planes . BMG has high glass-forming ability, good castability, good printability and unique characteristics The . Since past data is not available in the literatures for this BMG, its pair correlation function is theoretically generated from the interatomic pair potentials. A suitable, well-known and accepted model potential – Shaw’s constant core model potential is successfully exploited here for this investigation. Some of the important elastic and thermodynamic properties viz. Young’s modulus , modulus of rigidity Poisson’s ratio , Isothermal bulk modulus , , transverse sound velocity longitudinal sound velocity , , Debye-temperature are theoretically computed from PDCs of this BMG . 2. THEORETICAL METHODOLOGY A well-established Pseudo-Alloy Atom (PAA) model [1, 2] is adopted for investigating vibrational properties of BMG elucidation on Shaw’s constant core model potential is, . . (01) based BMGs are used to prepare complex shaped optical mirrors with smooth surface and good reflectivity with high dimensional accuracy. based BMGs are ideal materials for bio-medical applications because of their low density, higher biocompatibility and good corrosion resistivity. Here, al. (S) BMG is very first time theoretically investigated in terms of its elastic and thermodynamic properties through vibrational dynamics using pseudopotential theory [1,2]. In order to attain the phonon eigen frequencies, the two main computational approaches used have been developed by Hubbard-Beeby (HB) [4] and Takeno-Goda (TG) . The screening influence on the BMG properties has been studied by five local field correction functions viz. Hartree (H) [7], Taylor (T) [8], Ichimaru−Utsumi (IU) [9], Farid et al. (F) [10] and Sarkar et here, Z is valence, q is the wave vectors and volume. The model potential parameter is atomic can be obtained by fitting either to some experimental data or to realistic form-factors or other data relevant to the properties investigated. The pseudopotential parameter is so fixed that it may generate a pair correlation functions accurately consistent with the experimental data found in the literature. Instead of Vegard’s law, the electron-ion interactions are explained by PAA model . The ternary BMG system where p, q, and r are the proportionate concentration of the concerned element, is like a multi-component fluid containing bare ions and mixed ions immersed in a uniform electron gas. If the pair potentials of the single components @ IJTSRD | Unique Reference Paper ID – IJTSRD21550 | Volume – 3 | Issue – 2 | Jan-Feb 2019 Page: 1076 International Journal of Trend in Scientific Research and Development (IJTSRD) @ www.ijtsrd.com eISSN: 2456-6470 are known, the mean effective density dependent interatomic pair potential V(r) can be derived successfully . Here, the fundamental component pair potential is given by, arises from repulsion of the d-electron muffin- tin orbitals on different sites due to their non-orthogonality. Wills and Harrison studied the effects of the s-band and d-band. (02) . The contribution from the s-electron to the pair potential is then, (03) Where, Here, Where, (05) is the local field correction function, and are mass and charge of an electron respectively For BMG, the model potential parameter [1, 2, 15] is given below. (06) is the core radius. The number of s-valance electron is obtained by integrating the partial S- density of states, which result from the self-consistent band structure computation for the entire series and series. The number of d-electrons contributing to the pair-potential is . The d-state radii and the nearest neighbor coordinate number N are given by , Where, is the Wigner Seitz radius of the BMG. The input parameters of s-electron valance (ZS), d-electron valance (Zd), d-band radius (Rd), Wigner-Seitz radius (RS), Volume ( ), Coordination. No. (N), Mass (M) and Core radius (Rc) are used for computation and tabulated in table: 1. (04) Table 1: Input parameters and Constants useful in the computational work. M 3.32 The parameters , , 1.50 1.65 1.45 1.9465 and N are determined from band structure data of pure metallic component which are already found in the literature [1, 2, 15] and obtained by the following expressions. (07) 102.56 7.92 of rigidity 67.54 0.6654 , Poisson’s ratio and the Debye temperature are derived by the formulae [1, 2] given below. (13) (14) (08) (09) N= , , (10) is valency. The PCF (15) is as important as the interatomic pair potential V(r) in studying a BMG [1, 2, 16]. (11) Where, is Room temperature and (16) , the Boltzmann’s (17) constant. The mathematical notations and theoretical discussions are found from the respective papers of HB- and TG- approaches . In the long wavelength limit of the phonon frequency spectrum, the longitudinal and transverse frequencies are proportional to the wave vectors. and . (12) The longitudinal and transverse sound velocities ( and respectively) are computed from the long-wavelength limits of the PDCs as given in the literatures [1, 2, 4-6]. Young’s modulus , Isothermal bulk modulus , Modulus Here, is the Debye frequency, is isotropic number density. 3. RESULTS AND DISCUSSION: Figures 1 and 2 show the PDCs of for longitudinal and transverse modes of phonon eigen frequencies ( and ) versus wave vector computed with HB− and TG− approaches respectively with the ive local ield screening functions Viz. H, T, IU, F and S. The obtained phonon dynamical or vibrational properties for this BMG can be compared with the other such and experimentally generated data whenever available. @ IJTSRD | Unique Reference Paper ID – IJTSRD21550 | Volume – 3 | Issue – 2 | Jan-Feb 2019 Page: 1077 International Journal of Trend in Scientific Research and Development (IJTSRD) @ www.ijtsrd.com eISSN: 2456-6470 The inclusion of exchange and correlation effect increases the phonon eigen frequencies for both longitudinal and transverse modes. For the HB-approach, the plot of T-, S- and F- screening functions are lying between those due to H- and IU-screening functions for both branches. In TG-approach, the plots of H-, T- and F-are lying between those of S- and IUfunctions for both branches. The first minimum for the longitudinal frequency the HB-approach, is found around at and for H- T-, IU- F- and S- functions respectively. Typically, the dispersion relations express a minimum near , the wave-vector where the static structure factor of the BMG has its first maximum. The first maximum for the longitudinal frequency in the HB-approach is found around at in approach, it is found around at for H- function, for H- for T- IU and F- functions and for the rest of the functions; in the TG- approach, it is found around for all functions; in the TG- for S-function. and In the HB approach, the first minimum transverse frequencies for all functions are found around while in TG approach, it is found at respectively for the H-, T-, IU-, F- and S- functions. For the transverse branch and the first maximum is found around at for F- ; for the rest of local field correction functions in HB- approach, In the TG approach, it is found around at and for H-, T, IU-, F- and S-functions respectively. @ IJTSRD | Unique Reference Paper ID – IJTSRD21550 | Volume – 3 | Issue – 2 | Jan-Feb 2019 Page: 1078 International Journal of Trend in Scientific Research and Development (IJTSRD) @ www.ijtsrd.com eISSN: 2456-6470 Figure : PDCs of longitudinal and transverse Phonon frequencies for The first crossover position of and functions. The first crossover position of BMG using HB approach. in the HB-approach is observed at and for all local field correction in the TG-approaches is seen at and for H, T-, IU- and F- and S- functions respectively These both PDCs collectively disclose that the longitudinal mode oscillations are more prominent than that of the transverse one. The instability of the transverse mode oscillations is due to anharmonicity of the atomic vibration in the BMG system. The collective excitations at larger momentum transfer is because of the prominence of longitudinal mode vibrations only. Table2: Elastic and Thermodynamic properties of App. HB-approach TG-approach BMG. SCR H T IU F S H T IU F S K σ 2.62 3.59 3.79 3.78 2.85 2.67 2.47 2.69 2.69 2.07 1.51 2.07 2.19 2.18 1.65 0.99 1.01 1.09 1.09 0.82 1.69 3.18 3.54 3.52 2.00 2.59 2.10 2.52 2.51 2.57 1.02 1.91 2.12 2.11 1.20 0.43 0.45 0.52 0.53 0.51 0.25 0.25 0.25 0.25 0.25 0.42 0.40 0.40 0.40 0.41 @ IJTSRD | Unique Reference Paper ID – IJTSRD21550 | Volume – 3 | Issue – 2 | Jan-Feb 2019 2.54 4.77 5.30 5.29 3.00 1.23 1.27 1.47 1.48 1.44 200.46 274.71 289.60 289.08 217.96 133.76 136.66 146.89 147.45 126.67 Page: 1079 International Journal of Trend in Scientific Research and Development (IJTSRD) @ www.ijtsrd.com eISSN: 2456-6470 4. CONCLUSION: It is concluded that the phonon dynamics of BMG can be estimated by the PDC generated form HB- and TG- approaches with five local field correction functions, due to H-, T, IU-, F- and S-, with the successful application of the Shaw’s model potential, produce all broad characteristics of the dispersion curves and predict for the various useful thermodynamic and elastic properties under investigation. . The computed PDCs show extensive features of broad range collective excitations in BMG. The dielectric function is significant in the computation of the screening potential due to electron gas and the local filed correction functions. The relative effects of exchange and correlation in the selected properties, examined by different local field correction functions, show variations according to the vibrational properties. The thermodynamic properties obtained due to BS-approach are higher than those due to HB or TG-approaches. The complete picture tells the importance of local field correction function as well as the approaches in analysing the properties of the BMG. Since the experimentally or theoretically observed data of most of this BMG are not available in the literature, it is difficult to make any special remarks. However, this investigation proves to be very useful to offer vital information concerning a particular BMG system. References: [1] A. M. Vora, Vibrational Dynamics of Binary Metallic Glasses, Lap Lambert Academic Publishing, Germany (2012). [2] A. M. Vora, Vibrational Dynamics of Bulk Metallic Glasses Studied By Pseudopotential Theory, Computational Materials, Ed. Wilhelm U. Oster, Nova Science Publishers, Inc., New York (2009), pp.119-176. [3] A. Inou, X.M. Wang and W. Zhang, Rev. Adv. Mater. Sc., Vol. 18, (2008), pp. 1-9. [5] S. Takeno; M. Goda, Prog. Thero. Phys., (1971), Vol. 45, pp. 331-352. [6] S. Takeno; M. Goda, Prog. Thero. Phys., (1972), Vol. 47, pp. 790-806. [7] W. A. Harrison, Elementary Electronic Structure, (1999), World Scientific, Singapore. [8] R. Taylor, J. Phys. F: Met. Phys., (1978), Vol. 8, pp. 16991702. [9] S. Ichimaru; K. Utsumi, Phys. Rev. B., (1981), Vol. 24, pp 7385-7388. [10] B. Farid; V. Heine; G. Engel, I. Robertson, J. Phys. Rev. B. (1993), Vol. 48, pp.11602-11621. [11] A. Sarkar; D.S. Sen; S. Haldar; D.Roy, Mod. Phys. Lett., B. (1998), Vol. 12, pp. 639-648. [12] R.W.Shaw, Phy. Rev., (1968), Vol. 174, p. 769. [13] Gupta A.; Bhandari D.; Jain K. C.; Saxena N. S. Phys. Stat. Sol. (b). Vol. 95, (1996), pp. 367-374. [14] W. A. Harrison, Pseudopotentials in the Theory of Metals, (1966), W. A. Benjamin, Inc., New York. [15] J. M. Wills; W.A. Harrison, Phys. Rev B., (1983), Vol. 28, pp. 4363-4373. [16] E. TFaber, Introduction to the Theory of Liquid Metals; (1972), Cambridge Uni. Press: London. [17] V. Heine and D. Weaire, Solid State Physics 24, Eds. H. Ehrenreich, F. Seitz and D. Turnbull, Academic Press, New York (1970) p.249. [18] L. I. Yastrebov and A. K. Katsnelson, Foundations of One-Electron Theory of Solids, (1987), Mir Publications, Moscow. [19] J. M. Ziman, Principal of the theory of the solids, 2nd edition, (1972), Cambridge Uni. Press, London. [4] J. Hubbard; J. L. Beeby, J. Phys. C: Solid State Phys, (1969), Vol. 2, pp. 556-571. @ IJTSRD | Unique Reference Paper ID – IJTSRD21550 | Volume – 3 | Issue – 2 | Jan-Feb 2019 Page: 1080